#------------------------------------------------------------------------------
#$Date: 2016-02-18 14:25:00 +0200 (Thu, 18 Feb 2016) $
#$Revision: 176728 $
#$URL: svn://www.crystallography.net/cod/cif/8/10/16/8101644.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_8101644
loop_
_publ_author_name
'Zheng, Yue-Qing'
'Peters, Karl'
'von Schnering, Hans Georg'
_publ_section_title
;
Crystal structure of dithallium(I) octa-μ₃-bromohexabromo-
octahedro-hexatungstate(2-), Tl₂[(W₆Br)Br]
;
_journal_issue                   4
_journal_name_full
'Zeitschrift für Kristallographie - New Crystal Structures'
_journal_page_first              681
_journal_page_last               682
_journal_volume                  213
_journal_year                    1998
_chemical_formula_structural     'Tl2 [W6 Br8] Br6]'
_chemical_formula_sum            'Br14 Tl2 W6'
_chemical_formula_weight         2630.58
_space_group_IT_number           201
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-P 2ab 2bc 3'
_symmetry_space_group_name_H-M   'P n -3 :2'
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            4
_cell_length_a                   13.873(2)
_cell_length_b                   13.873(2)
_cell_length_c                   13.873(2)
_cell_measurement_temperature    293(2)
_cell_volume                     2670.0(7)
_diffrn_ambient_temperature      293(2)
_exptl_crystal_density_diffrn    6.544
_refine_ls_R_factor_obs          0.0478
_refine_ls_wR_factor_obs         0.1042
_cod_original_sg_symbol_H-M      'P n -3'
_cod_database_code               8101644
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x+1/2, -y+1/2, z'
'-x+1/2, y, -z+1/2'
'x, -y+1/2, -z+1/2'
'z, x, y'
'z, -x+1/2, -y+1/2'
'-z+1/2, -x+1/2, y'
'-z+1/2, x, -y+1/2'
'y, z, x'
'-y+1/2, z, -x+1/2'
'y, -z+1/2, -x+1/2'
'-y+1/2, -z+1/2, x'
'-x, -y, -z'
'x-1/2, y-1/2, -z'
'x-1/2, -y, z-1/2'
'-x, y-1/2, z-1/2'
'-z, -x, -y'
'-z, x-1/2, y-1/2'
'z-1/2, x-1/2, -y'
'z-1/2, -x, y-1/2'
'-y, -z, -x'
'y-1/2, -z, x-1/2'
'-y, z-1/2, x-1/2'
'y-1/2, z-1/2, -x'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_thermal_displace_type
_atom_site_occupancy
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_disorder_group
W W 0.12378(5) -0.03176(5) 0.04283(5) 0.0330(2) Uani 1 d . .
Br1 Br 0.13439(12) 0.13439(12) 0.13439(12) 0.0511(8) Uani 1 d S .
Br2 Br 0.19684(12) 0.04796(13) -0.11312(13) 0.0427(4) Uani 1 d . .
Br3 Br 0.29692(13) -0.0771(2) 0.09958(15) 0.0586(6) Uani 1 d . .
Tl1 Tl 0.5000 0.0000 0.0000 0.0548(5) Uani 1 d S .
Tl2 Tl 0.2500 0.7500 0.7500 0.0641(8) Uani 0.67 d SP .
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
W Br3 2.605(2) . ?
W Br2 2.618(2) 17 ?
W Br2 2.633(2) . ?
W Br2 2.635(2) 9 ?
W Br1 2.636(3) . ?
W W 2.6434(12) 5 ?
W W 2.6435(12) 9 ?
W W 2.6448(12) 21 ?
W W 2.6449(12) 17 ?
Br1 W 2.636(3) 5 ?
Br1 W 2.636(3) 9 ?
Br2 W 2.618(2) 21 ?
Br2 W 2.635(2) 5 ?
Br3 Tl2 3.245(2) 17_656 ?
Tl2 Br3 3.245(2) 21_566 ?
Tl2 Br3 3.245(2) 22_666 ?
Tl2 Br3 3.245(2) 23_566 ?
Tl2 Br3 3.245(2) 24_666 ?
